**HAL Id: tel-03219512**

**https://tel.archives-ouvertes.fr/tel-03219512**

Submitted on 6 May 2021

**HAL is a multi-disciplinary open access**

archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Combining RBS/Channeling, X-ray diffraction and**

**atomic-scale modelling to study irradiation-induced**

**defects and microstructural changes**

### Xin Jin

**To cite this version:**

Xin Jin. Combining RBS/Channeling, X-ray diffraction and atomic-scale modelling to study irradiation-induced defects and microstructural changes. Materials. Université de Limoges, 2021. English. �NNT : 2021LIMO0017�. �tel-03219512�

### UNIVERSITÉ DE LIMOGES

### École Doctorale Sciences et Ingénierie des Matériaux, Mécanique,

### Énergétique (ED 609)

### Institut de Recherche sur les Céramiques (IRCER)

Année : 2021

### Thèse

pour obtenir le grade de

### DOCTEUR DE L'UNIVERSITÉ DE LIMOGES

Discipline : Physique

présentée et soutenue par

### Xin JIN

le 24 02 2021

### Combining RBS/Channeling, X-ray

### diraction and atomic-scale modelling to

### study irradiation-induced defects and

### microstructural changes

Thèse dirigée par Alexandre Boulle et Aurélien Debelle

JURY :

Patrice Gergaud Directeur de Recherche, CEA LETI, Grenoble Rapporteur

Katharina Lorenz Principal Researcher, Universidade de Lisboa Rapporteur

Marie-France Barthe Directeur de Recherche, CNRS, CEMTHI, Orléans Examinatrice (Président) Jacek Jagielski Professor, National Centre for Nuclear Research, Poland Examinateur

Aurélien Debelle Maître de Conférences, IJCLab, Orsay Examinateur

Alain Chartier Directeur de Recherche, CEA Saclay Examinateur

S = kBlnΩ

L. Boltzmann

### Acknowledgments

First, I would like to express my gratitude to my two supervisors, Dr. Aurélien Debelle and Dr. Alexandre Boulle, without whom it is not possible to nish this thesis work. My work with Dr. Aurélien Debelle started from my M2 internship in Orsay. Since then, he led me into the eld of research, and taught me general knowledge for almost all the techniques or methods which I encountered in my PhD. He is always very kind and patient when we have discussions and when he exams my manuscripts. His enthusiasm inspired me to always keep a positive mindset, which provides an important impetus to overcome challenges. I systematically studied XRD from Dr. Alexandre Boulle in Limoges. I have only stayed there during a relatively short period. But it is amazing that he managed to teach me XRD theories, experiments and computations in a very complete and clear way. I also learned a lot from his computer programs. In addition, both of my supervisors provided me strong support no matter in the scientic eld or in other elds, for which I am very grateful.

Special and sincere thanks to my team members. Especially, Prof. Frédérico Garrido and Prof. Lionel Thomé are very friendly and helped me a lot in terms of understanding RBS/C as well as ion/solid interactions. Dee Jay Cerico provided constant help for almost three years.

I would like to thank my collaborators, including Dr. Jean-Paul Crocombette, Dr. Alain Chartier, Dr. Flyura Djurabekova, Prof. Kai Norlund and Dr. Shuo Zhang. Dr. Jean-Paul Crocombette almost participated to all of my thesis work. His help is instrumental for the studies related to RBS/C simulations and radiation eects in Fe. He can always pinpoint important factors. Dr. Alain Chartier provided important data related to the study of radiation eects in UO2, which is one of the foundations of this

thesis work. Dr. Flyura Djurabekova, Prof. Kai Norlund and Dr. Shuo Zhang provided valuable help in terms of RBS/C simulations, which strongly facilitated my work.

I would also like to thank Prof. Jacek Jagielski and Dr. Lech Nowicki for the discussions related to RBS/C simulations.

Many thanks to SCALP facility sta for their assistance, the lab of IJCLab (CSNSM), the PHINIICS and SIMME doctoral schools.

## Contents

List of acronyms 3

Introduction 5

1 Particle-solid interactions and radiation eects 9

1.1 Ion-solid interactions . . . 9

1.1.1 Nuclear energy loss . . . 9

1.1.2 Electronic energy loss . . . 18

1.2 Other particle-solid interactions . . . 21

1.2.1 Neutron irradiations . . . 21

1.2.2 Electron and photon irradiations . . . 23

1.3 Radiation eects . . . 24

1.3.1 Primary radiation damage . . . 25

1.3.2 Defect evolution and other radiation eects . . . 31

2 Characterization techniques 36 2.1 Rutherford backscattering spectrometry in channeling mode . . . 36

2.1.1 Basic theory . . . 36 2.1.2 Applications . . . 42 2.2 X-ray diraction . . . 46 2.2.1 Basic theories . . . 46 2.2.2 Applications . . . 50 2.2.3 Simulations . . . 53

3 Simulations of RBS/C spectra of irradiated materials 58 3.1 MC-RBS/C simulation methods . . . 58

3.1.1 RBSADEC . . . 61

3.2 Improvement of RBS/C simulations . . . 63

3.2.1 Simulations of random spectra . . . 64

3.2.2 Target atomic thermal vibrations . . . 71

3.2.3 Incident ion beam divergence . . . 74

3.2.4 Simulation of aligned spectra . . . 77

3.3 Discussion and summary . . . 80

4 Combination of RBS/C and XRD with molecular dynamics to investigate radiation eects in materials 81 4.1 Simulation methods: UO2 . . . 81

Contents

4.1.2 Analysis of defects . . . 83

4.1.3 XRD and RBS/C methods . . . 85

4.2 Characterization of radiation damage: UO2 . . . 88

4.2.1 Strain kinetics . . . 88

4.2.2 Disordering kinetics . . . 92

4.3 Systematic study of model defective systems - Fe as a test-case . . . 98

4.3.1 Description of model defective systems . . . 98

4.3.2 Systematic study of model defective systems: Fe . . . 101

4.4 Summary . . . 119

Conclusions and perspectives 120

Appendices 123

A Dechanneling fractions in RBS/C spectra generated from UO2 MD cells123

B Models of the disorder build-up 126

List of acronyms

### List of acronyms

1D one-dimensional 2D two-dimensional 3D three-dimensional

arc-dpa athermal recombination corrected displacements per atom ASD Alternative slowdown

BCA Binary collision approximation BCC Body-center cubic

BK Brandt-Kitagawa

CDF Cumulative distribution function CM Center of mass

dpa displacements per atom DXA Dislocation analysis DW Debye-Waller

EAM Embedded-atom method FCC Face-centered cubic FFP Free ight path

FFT Fast Fourier transform FMD Freely migrating defect FP Frenkel pair

FPA Frenkel pair accumulation GPU Graphical processing unit HBS High burn-up structure HEI High energy ion

IBD Ion beam divergence Lab Laboratory

LEI Low energy ion

List of acronyms

KMC Kinetic Monte Carlo KP Kinchin and Pease MC Monte Carlo

MD Molecular dynamics

MSDA Multi-step damage accumulation NRT Norgett, Robinson and Torrens

NVE Number of particles, volume and energy PDF Probability density function

PIPS Passivated implanted planar silicon PKA Primary knock-on atom

PSA Planar scattering approximation PWR Pressurized water reactor

RBS Rutherford backscattering spectrometry

RBS/C Rutherford backscattering spectrometry in channeling mode RDA Randomly displaced atom

RE Rate equation

r.l.u reciprocal lattice unit rms root mean square

RMSD root-mean-square deviation RSM Reciprocal space map

SHI Swift heavy ions SIA Self interstitial atom

SP-CSA Single-phase concentrated solid solution alloy TDDFT Time-dependent density functional theory TEM Transmission electron microscopy

XRD X-ray diraction

YSZ Yttria-stabilized zirconia ZBL Ziegler-Biersack-Littmark

## Introduction

For most of human history, apart from light, people's lives are basically free from the radiation eect of energetic particles, despite the fact that these kinds of particles are pervasive in our solar system, e.g., ions in the solar wind. These ions are mainly composed of H and He with trace amount of heavier elements [1], and their average energy is around 1 keV/nucleon [2]. Due to the existence of Earth's magnetosphere, both ions and electrons in the solar wind are deected away, and thus exert little inuence on human society except by making people wondering at some spectacular phenomena induced by them, for example, aurorae [3, 4] and comet tails [5, 6].

However, in the modern society, there is an increasing number of activities involving the use of energetic particles; these later include ions, neutrons, electrons and photons. One important example is the ion irradiation used in several industry and research elds that have beneted greatly from the introduction of foreign atoms and modication of the target atomic structure. Ion implantation can be used for the doping of semiconductor materials, which is one vital step for modern integrated-circuit manufacturing [7, 8] and can have potential applications in novel optoelectronic devices as well [9]. In the eld of nanoscience, ion irradiation keeps drawing attention due to the fact that it can be used to change the atomic structure of nanomaterials in a controlled manner [1012] and to tailor various properties of nanomaterials including mechanical, electrical and magnetic properties [1315]. In the nuclear industry, in order to eectively predict material behaviors in both ssion and fusion nuclear reactors, a considerable amount of eort has been made to emulate reactor irradiation with ion irradiation due to the following advantages of the latter over the former: higher safety and accessibility, faster damage production and lower cost of post-irradiation characterization [1618]. A last but not the least example of the application of ion irradiation lies in the eld of astronomy, where the information related to the concentration of implanted ions and the degree of structure modication can be used to estimate the age or lifetime of the object directly exposed to the bombardment of energetic particles [1921], and relevant irradiation-induced eects can be critical to some intriguing questions, for example, the possible origin of H2O on

Introduction

Apart from these benets, the irradiation by energetic particles can often be detrimental to materials when their structures are modied in undesirable ways. This has produced a profound eect on the development of the nuclear materials bearing intense bombardment of particles generated during nuclear reactions. The amount of radiation damage in materials can be quantied by a commonly used parameter called displacements per atom (dpa); a damage level of 1 dpa means that, on average, each atom in the material has been permanently displaced from its original position once. In pressurized water reactors (PWR), which accounted for 66 % of operational reactors worldwide by the end of 2018 [24], the dpa value in in-core structural materials can be as high as 80 dpa [25]. The consequence of the high level of radiation damage is the signicant deterioration of material properties. For example, reactor irradiation can degrade the fracture toughness of materials [26], which may result in structure failure under nominal operational conditions; it can also cause dimensional changes due to swelling and creep [27], which is able to hinder the normal operation of reactor components; under harsh environment in nuclear reactors, incidents of intergranular cracking in reactor components have been reported as being due to a complex mechanism called irradiation assisted stress corrosion cracking [28, 29], which poses potential risks on the reactor integrity.

Due to the degradation of materials induced by reactor irradiation, the lifetime of current operational reactors are limited accordingly, and subsequently the economics of nuclear power plants are aected, since capital costs, e.g., construction costs, make up a large part of total nuclear electricity generation costs [30]. Moreover, material behaviors under irradiation are posing great challenges for the safety of generation IV nuclear reactors [31] and future fusion reactors [32]. This is not only due to the higher irradiation dose in some of the more advanced reactors, but also because almost all these advanced reactors will operate in harsher environments as compared to those in current generation II and III reactors [33]. The coupling of intense irradiation with other extreme environments, for example, high temperature, can amplify additional deterioration mechanisms of materials, such as, high temperature helium embrittlement [34, 35].

In addition to the eld of nuclear energy, radiation eects can also play deleterious roles in other elds, for example, defect production during ion doping [36], electrical properties degradation of detectors [37], thermoelectric properties degradation of devices in space [38], etc. Therefore, in order to develop materials with excellent irradiation-resistance ability as well as to further explore the usage of particle irradiation, it is crucial to have a comprehensive understanding of the underlying mechanisms of irradiation-induced eects in general, and of defects in particular.

Introduction

Experimental studies of radiation eects in solid materials date back to the middle of the nineteenth century [39], when sputtering due to glow discharges was observed [40]. Currently, radiation damage is extensively characterized by directly identifying the defects induced by irradiation, using for instance transmission electron microscopy (TEM) [41], and by monitoring phenomenological parameters related to radiation damage levels obtained from techniques including, but not limited to, Rutherford backscattering spectrometry in channeling mode (RBS/C), X-Ray diraction (XRD), Raman spectroscopy and positron annihilation spectroscopy [42]. In some cases, the phenomenological parameters can be directly used to quantify certain physical changes such as the amorphization process. In some situations, the disorder build-up (disorder versus irradiation dose) obtained from these phenomenological parameters can allow identifying the defects at the origin of the damage, provided that several complementary techniques (with dierent sensitivity to dierent defects) are combined.

In parallel with experiments, computational studies have been devoted to simulating
the generation and evolution of radiation defects [43]. From atomistic levels, the initial
stages of radiation eects, i.e., production of primary damage, can be eectively simulated
by molecular dynamics (MD) simulations. However, conventional MD simulations are
limited in time scale (∼ 102 _{− 10}3 ps) as well as in size scale (depending on computer

capacities) [44]. For simulating damage evolution after the stage of primary damage, the tasks have to be delivered to other methods or techniques, e.g., the rate equation (RE) method, Kinetic Monte Carlo (KMC) simulations, etc. Yet, if the thermal migration of defects on large time scale is neglected, conventional MD simulations can still be used to mimic damage evolution induced by high doses irradiation. One method is to simulate overlaps of collision cascades induced by recoils [45,46]; another one is to directly introduce defects, resulted from the primary damage (e.g. Frenkel pairs (FPs)), into MD cells [47, 48]. In terms of the characterization of radiation eects from simulated targets containing atomic information, numerous computational methods have been developed to identify radiation defects including point defects, dislocations, amorphous clusters, etc [4951]. Nevertheless, signals from experimental characterization techniques have not yet been extensively produced from such computed targets. For example, the computational method which is able to generate RBS/C signals from MD cells was not developed until recently [52]. Thus, new insights on radiation eects are expected to be obtained from the simulation of the characterization technique signals, if they rely on perfectly known, computationally-generated data.

In this thesis, we will present a work dedicated to studying radiation damage in materials by combining computational and experimental RBS/C and XRD signals. Both techniques are currently used to estimate disorder parameters and the elastic strain (with

Introduction

XRD only), and have the advantage of generating little or no damage in targets. It is of interest to integrate the computational and experimental approaches by simulating signals recorded during characterization experiments due to the following reasons: (i) the comparison of computational and experimental results can be utilized to evaluate the validity of computational simulations; (ii) it provides an ecient way to establish direct connections between defects and phenomenological parameters, since most experimental characterization techniques do not allow direct observation of defects (except using some often destructive and lengthy methods [53]); such connections are essential for the interpretation of experimental data.

Uranium dioxide (UO2) is chosen as an example target for this approach. Indeed,

as it is the most widely used nuclear reactors fuel, the radiation eects in this material have been extensively investigated, both experimentally and computationally [54], which provides benchmarks for testing our methodology. Besides, UO2targets containing various

irradiation-induced defects have been recently generated by MD simulations using the FP accumulation method [55], which can serve as input data set for generating RBS/C and XRD signals. The investigation of radiation eects will be focused on the build-ups of disorder and elastic strain in damaged UO2. In addition, to this specic work, a

systematic investigation of Fe targets (each containing one single type of defects created by MD simulations) will also be presented. In the study using Fe targets, we will rst give a description of the eect of dierent types of defects on elastic strain and disorder, and then present the variation of RBS/C signal as a function of He energy and its implication on defect types.

The thesis manuscript is organized into four chapters. In the rst chapter, the basic theories of particle-solid interactions and the consecutive potential radiation eects are briey presented. The second chapter recalls the basic principles of the RBS/C and XRD techniques. The third chapter focuses on the development of a RBS/C simulation program. In the fourth chapter, we rst address the RBS/C and XRD simulation results from damaged UO2 targets and studies on the build-ups of disorder and of elastic

strain, and then provide results of the systematic study of Fe targets. Conclusions and perspectives are given at the end.

## Chapter 1

## Particle-solid interactions and radiation

## eects

In irradiation processes, both the fate of incident particles and the origin of radiation eects in solid materials are decided by how the particles interacts with target atoms. In this chapter, we will rst present the basic theories of particle-solid interactions, with a particular focus on ion-solid interactions. Interactions due to other types of incident particles, including neutrons, electrons and photons, will also be briey mentioned. Then, we will present how the bombardment of energetic particles gives rise to radiation eects.

### 1.1 Ion-solid interactions

As an energetic ion penetrates a target, it loses its energy through collisions with target atoms. At least since Bohr's work in the 1940s [56], it is customary to consider the energy loss process by distinguishing elastic collisions with target atoms and interactions with target electrons resulting in atomic excitations or ionizations. The energy loss due to the former mechanism is referred to as nuclear energy loss, and the energy loss due to the latter one is referred to as electronic energy loss. In the following, we shall follow this convention and we will show how to get essential understanding of the rather complex interaction processes which involve numerous variables, mainly based on classical mechanics.

### 1.1.1 Nuclear energy loss

The information about the nuclear energy loss is obtained by studying the kinematics of elastic collisions [57]. In an elastic collision, normally, only two isolated particles, namely the moving ion and an initially resting target atom, are involved. Fig.1.1(a) depicts such a collision in the laboratory (Lab) reference frame, in which the ion with a mass of M1 is represented by the black solid circle and the target atom with a mass of

Chapter 1. Particle-solid interactions and radiation eects

M2 is represented by the blue solid circle. The black and blue dashed circles represent

the initial positions of the ion and atom, respectively.

(a) Lab

(b) CM

Figure 1.1 Illustrations of binary collisions in the (a) Lab and (b) CM reference frames. The dashed lines are asymptotic lines of the actual trajectories (solid lines) of the ion (black circle) and atom (blue circle).

Conservations of particles energy and momentum can be expressed by the following

Chapter 1. Particle-solid interactions and radiation eects equations: 1 2M1v 2 0 = 1 2M1v 2 1+ 1 2M2v 2 2 (1.1a) M1v0 = M1v1cos θ + M2v2cos φ (1.1b) 0 = M1v1sin θ − M2v2sin φ (1.1c)

where v0 is the initial energy of the ion, v1 is the ion energy after the collision, v2 is the

atom energy after the collision, θ is the ion scattering angle and φ is the atom scattering angle. From Eq.(1.1), we can get the kinematic factor, k, which is the ratio of the scattered energy of ion to the initial energy of ion, E0:

k = M1cos θ ±
p
M2
2 − M12sin
2_{θ}
M1+ M2
!2
(1.2)

Eq.(1.2) can be often found useful in Rutherford backscattering experiments, in which the plus sign should be taken, because the term of backscattering indicates M1 < M2.

The energy transferred to the target atom, T , can also be calculated from Eq. (1.1). If the Lab frame can be changed into a center of mass (CM) reference frame as shown in Fig.1.1(b), then the transferred energy T can be expressed in a more concise form which is as follows: T = TMsin2 θc 2 = 4M1M2 (M1+ M2)2 E0sin2 θc 2 (1.3)

where TM is the maximum transferable energy in a head-on collision, θc is the ion

scattering angle in the CM system. In Fig.1.1(b), θc+ φc = π, and the center of mass,

which is the origin point in the CM frame, is denoted by the orange dot.

While the scattering angles in the equations above are implicitly indicated as known
values, this is not the case in most of the conditions. Here we present two popular
approaches for calculating the scattering angle and show how its examination leads to the
concepts of collision cross section and stopping power. The rst approach is to solve the
classical scattering integral, and the second one is based on the impulse approximation1_{.}

Approach of the classical scattering integral

The rst method is to calculate the classical scattering integral. In the CM system, the velocity of ion or atom can be decomposed into a radial (towards the origin) and a

1_{The scattering angle can also be calculated analytically using the so-called Magic formula, in which}
tting parameters are decided by comparing results with those obtained from the classical scattering
integral [58].

Chapter 1. Particle-solid interactions and radiation eects

transverse component. Thus, the total kinetic energy of the ion and atom reads:

EKE =
1
2M1
"
dr1
dt
2
+ r2_{1} dΘc
dt
2#
+1
2M2
"
dr2
dt
2
+ r_{2}2 dΘc
dt
2#
(1.4)

in which r1 is the distance from the ion to the origin, r2 is the corresponding distance

for the atom, and Θc is the angle between the line r and the line perpendicular to the

shortest line connecting the ion and atom in the collision, rmin as give in Fig.1.1(b). By

considering the fact that r1+ r2 = r and r1/r2 = M2/M1, Eq.(1.4) can be converted to:

EKE = 1 2Mc " dr dt 2 + r2 dΘc dt 2# (1.5)

where Mcequals to (M1M2)/(M1+M2). From Eq.(1.5), we see that the two-body problem

can be replaced by the study of one equivalent particle with the reduced mass as Mc

moving about a xed center of force, which simplies ensuing calculations. According to the property of the CM system, the total energy in that system, Ec, can be represented

by:

Ec= EKE + V (r) =

M2

M1+ M2

E0 (1.6)

where V (r) is the potential energy. Taking into account the energy conservation represented by Eq.(1.6) and the conservation of the angular momentum (which equals to Mcr2(dΘc/dt)), the rate of change of the angle Θc over r, dΘc/dr, can be obtained,

from which the scattering angle is derived as:

θc= π − 2b
Z ∞
rmin
dr
r2_{[1 −}V (r)
Ec − (
b
r)2]1/2
(1.7)

where b is the impact parameter. Eq.(1.7) indicates that the scattering angle is a function of the impact parameter b, total energy Ec and interatomic potential energy V (r).

The potential used in Rutherford backscattering experiments, i.e., the Coulomb potential, can be expressed by:

V (r) = e

2_{Z}
1Z2

r (1.8)

where e2 _{= 1.44}_{eV·nm}2_{, Z}

1 is the atomic number of the ion and Z2 is the atomic number

of the target atom. Using the Coulomb potential, the scattering angle is calculated as
follows:
sin2 θc
2 =
α2
α2 _{+ (2E}
cb)2 (1.9)

2_{The constant e}2 _{used in this work is in the cgs unit, in which the Coulomb law constant 1/4(π}
0)is
equal to 1 where 0 is the vacuum permittivity

Chapter 1. Particle-solid interactions and radiation eects

in which α = Z1Z2e2. While the use of the Coulomb potential can be valid when the

interatomic distance is small, in most cases, we need to take into account the screening of the nucleus by its surrounding electrons. Such screening eect can be introduced into the potential calculation by multiplying Eq.(1.8) with a screening function, χ(r). Depending on the form of the screening function used, Eq.(1.7) may not be able to be solved analytically, in which case numerical evaluations are required. A widely used screening function, namely, the universal screening function, χU, was developed by Ziegler,

Biersack and Littmark (ZBL), who performed the calculation by tting the interatomic potentials of 261 atom pairs [59]. The analytical form of χU is expressed as follows:

χU = 0.1818e−3.2x+ 0.5099e−0.9423x+ 0.2802e−0.4028x+ 0.02817e−0.2016x (1.10)

in which the reduced distance, x, is given by x = r/aU, where aU is the universal screening

length dened by:

aU =

0.8854a0

Z0.23

1 + Z20.23

(1.11) where a0 = 0.053 nm is the Bohr radius of the hydrogen atom. Thus, the universal

interatomic potential, VU, is expressed as:

VU(r) =

e2Z1Z2

r χU(x) (1.12) Generally, the higher the target atomic number Z2 is, the stronger the screening eect

will be.

Eq.(1.3), Eq.(1.7) and Eq.(1.12) can already provide accurate information for determining the trajectory of a single ion, if electronic collisions are temporarily neglected (which will be discussed in the next subsection). However, it is still interesting to see what kind of collective results, e.g., the stopping power, can appear due to a large number of interactions. For this purpose, we need to rstly evaluate probability-related quantities, namely, the angular and energy transfer cross sections.

The total angular cross section, σ(θc), can be represented by an area of πb2 in the

CM system, indicating that if the impact parameter is smaller than b, then the scattering angle of the ion will be greater than θc. The dierential angular cross section is produced

as follows: dσ(θc) dΩ = 2πbdb 2π sin θcdθc = b sin θc db dθc (1.13)

Chapter 1. Particle-solid interactions and radiation eects
[60] 3_{:}
dσ(θc)
dΩ =
α
4Ec
2
1
sin4(θc/2)
(1.14a)
dσ(θ)
dΩ0 =
e2_{Z}
1Z2
4E0
2
4[(M2
2 − M12sin
2_{θ)}1/2_{+ M}
2cos θ]2
M2sin4θ(M22− M12sin
2_{θ)}1/2 (1.14b)

where Eq.(1.14a) and Eq.(1.14b) use the notations in the CM and lab frames respectively, (dσ(θc)/dΩ)dΩ = (dσ(θ)/dΩ0)dΩ0 and θc= θ + arcsin(M1sin θ/M2). In parallel to σ(θc),

the total energy cross section, σ(E), indicates the probability for collisions to occur, where energy transfers are possible, when the ion energy is E. The dierential energy transfer cross section can be connected to the angular one through the following equation:

dσ(E) dT = 4π TM dσ(θc) dΩ = 4π TM b sin θc db dθc (1.15)

Now, we have almost all the tools to evaluate the stopping power. The average energy loss by the ion in an innitesimal distance is obtained by multiplying the transferred energy T with the probability of the collision to occur and then integrating over all possible T . Hence, the nuclear stopping power, which is the average energy loss per unit length, is expressed as follows:

dE dx n= N Z TM 0 Tdσ(E) dT dT (1.16)

where N is the target atomic density. Further, the nuclear stopping cross section, Sn, is

dened by dividing the nuclear stopping power by N. By converting the integration over
T in Eq.(1.16) into that over the impact parameter b, and applying reduced notations
[63], Sn is calculated as:
Sn(ε) =
ε
a2
U
Z ∞
0
sin2 θc
2db
2 _{(1.17)}

where ε = (aUEc)/αis the reduced energy which equals to the reduced distance aU divided

by the distance of closest approach. Using the scattering integral (Eq.(1.7)), Ziegler et al [59] numerically solved Eq.(1.17) and then proposed the following analytical tting

3_{This result based on classical mechanics happens to be the same with the result derived from quantum}
mechanics (e.g., based on the Born approximation [61]) except in one condition: If it is impossible to
distinguish the particles involved in the interaction, e.g., a collision between two identical particles, a
quantum-mechanical correction is needed [62]. However, in practice, if we can consider that the energy
distribution of the particles which we are dealing with basically follows the Maxwell-Boltzmann statistics,
then they do not act like identical particles, in which case there is no need to invoke the
quantum-mechanical correction.

Chapter 1. Particle-solid interactions and radiation eects
functions:
Sn(ε) =
0.5 ln(1 + 1.1383ε)
ε + 0.01321ε0.21226_{+ 0.19593ε}0.5, f or ε 6 30 (1.18a)
Sn(ε) =
ln(ε)
2ε , f or ε > 30 (1.18b)
in which the rst equation uses the universal interatomic potential, and the second one is
derived from the Rutherford backscattering4_{. Eq.(1.18) is applied in the widely used }

ion-solid interaction simulation code, SRIM [64]. As an example (chosen because it mimics an actual RBS/C experiment), the nuclear stopping power of He ions in UO2 is presented

in Fig.1.2, which increases with a higher energy in low energy regions and then decreases after reaching a peak (the electronic stopping powers in the gure will be presented in the following). For compound targets like UO2, the calculation of stopping powers follows

Bragg's rule [65] which states that the stopping power of a compound can be estimated by a weighted sum of the individual stopping powers.

Approach of the impulse approximation

Although accurate results can already be derived from the approach of the classical scattering integral, it is still interesting to present the approach of the impulse approximation due to the following reasons: (i) some methods used in the approach can be applied to calculate electronic stopping powers in the following; (ii) this approach provides a plausible physical reason about why nuclear stopping power decreases at high energy, which may be dicult to contemplate based on the scattering integral; (iii) the results obtained from this approach are still used by some calculation codes, such as DART [66,67].

The impulse approximation is used to treat small-angle calculations, in which the ratio of the potential energy to the kinetic energy Ec in the CM system remains small

through the entire collision process. In this approximation, we shall also only consider the trajectory of the equivalent particle with the mass as a reduced mass Mc as performed in

the case of the scattering integral. The initial and nal momentum of the particle are P1

and P2. The momentum change is 4P = P2− P1. As shown in Fig.1.3, in the limit of

4_{At rst glance, the introduction of new notations, i.e., reduced notations, may increase the complexity}
for understanding the results. However, the use of reduced notations decreases the number of variables,
for example, it enables to describe the nuclear stopping for all combinations of ion-atom collisions using
a single curve. Thus, it facilitates the comparison of results calculated from dierent methods, e.g., using
dierent interatomic potentials, and minimizes the necessary data to be stored in relevant simulation
codes.

Chapter 1. Particle-solid interactions and radiation eects

Figure 1.2 Stopping powers of He ions in UO2. The nuclear stopping power (blue

solid line) is calculated by SRIM. The electronic stopping powers are calculated by SRIM (orange solid line) and RUMP (green solid line). The blue dashed and dotted line is the t to the SRIM electronic stopping power in the low energy region, where the electronic stopping power increases with energy. Black lines are ts to the RUMP electronic stopping power. The inset shows the stopping powers in a log-log scale.

θc 1, the 4P follows following relation:

4p 2Mcv

∼_{=} θc

2 (1.19)

where v is the velocity of the equivalent particle. During the entire movement process of the particle, the component of the force acting on it, which is parallel to the incident direction, can be considered being balanced o. Hence, the change in momentum is only induced by the component of the force perpendicular to the incident direction, F0, which

is given by: 4P = Z ∞ −∞ F0dt = 1 v Z ∞ −∞ F0dx = 1 v Z ∞ −∞ −dV (r) db dx (1.20) Considering both the Eq.(1.19) and Eq.(1.20), the scattering angle in the impulse approximation can be calculated as:

θc= 1 Ec Z ∞ b dV dr b r " 1 − b r 2#−1/2 dr (1.21)

which has the same dependency on variables as Eq.(1.7).

Chapter 1. Particle-solid interactions and radiation eects

Figure 1.3 Illustrations of the trajectory of the equivalent particle with the mass as Mc.

Originally, the impulse approximation was meant for small-angle collisions. In order to apply the approximation in a more general condition, Lindhard et al [68] extrapolated the treatment to wide-angle collisions by replacing θc with 2 sin(θc/2) and replacing b2 with

b2 + b2_{0}, in which b2_{0} is an arbitrary constant. Then, using reduced notations, a universal
one-parameter dierential scattering cross section can be expressed as:

dσ = −πa

2

2

f (t1/2_{)}

t3/2 dt (1.22)

where a is a screening distance, f(t1/2_{)} is a function depending on the assumed form of

the screening function [69], and t is a dimensionless collision parameter dened by:

t = ε2 T TM

= ε2sin2θc

2 (1.23)

It can be found that t is a measure of the depth of penetration into the atom during a collision. Combining Eq.(1.16) and Eq.(1.23), the reduced nuclear stopping cross section can be given in a simple form:

Sn(ε) =
1
ε
Z ε
0
f (t1/2)dt1/2 (1.24)
Using this approximation, the stopping powers calculated from dierent interatomic
potentials 5_{, including the universal interatomic potential, can be calculated by adjusting}

tting parameters or forms of the function f(t1/2_{)} _{[}_{70}_{]. In addition, Eq.(1.20) indicates}

that the momentum change is related to the interaction time and thus related to the

5_{The potentials, which can be used in both the scattering integral and impulse approximation, should}
be spherically symmetrical.

Chapter 1. Particle-solid interactions and radiation eects

particle velocity. It is possible that if the velocity is higher than a certain value, the momentum change can be decreased due to shorter interaction time, which could be the reason for the decrease of the nuclear stopping power with a high incident energy.

### 1.1.2 Electronic energy loss

It is claimed that the subject was originally addressed by J. J. Thomson before the discovery of the atomic nucleus at the beginning of the last century [56, 71]. In contrast to the description of the nuclear energy loss, there is a lack of a single theoretical model which can accurately describe the electronic energy loss in a broad energy range mainly based on classical mechanics. The time-dependent density functional theory (TDDFT) method may provide the solution based on the rst principles [72, 73]. However, it is not in the scope of this thesis to describe the TDDFT method. In the following, we will show the mechanisms of the electronic stopping suitable for ions with low and high energies (or velocities), respectively [57], which is followed by a brief presentation of the empirical method used in SRIM.

Ions with low energies

The ions with low energies refer to the ions with velocity v smaller than v0Z 2/3

1 , where

v0 = 2.188 × 108 cm/s is the Bohr velocity. Qualitatively, for v < v0Z 2/3

1 , the ion is not

fully stripped of its electrons [74] and tends to neutralize by capturing electrons in target atoms. J. Lindhard, M. Schar and H. Schiott (LSS) [63,75] proposed that the electronic stopping power in this low energy region can be calculated as:

dE
dx
e= ξL8πe
2
a0N
Z1Z2
(Z_{1}2/3+ Z_{2}2/3)3/2
v
v0
(1.25)

where the correction factor ξL ∼= Z 1/6

1 . It can be found that the electronic stopping power

is proportional to v.

It was shown that this Lindhard form for electronic stopping can be explained by the Firsov model [57, 76]. In the Firsov model [77], because of the low ion velocity, the collision time between the ion and atom, which are represented by Thomas-Fermi atoms, is long enough for a fusion of the ion and atom into a quasi-molecule to occur. During the lifetime of this quasi-molecule, the electrons of both the ion and atom are able to exchange. When an electron in the atom is captured by the ion, the ion loses a small amount of momentum proportional to mev, in which me is the mass of the electron. Thus,

by examining the electron ux through the so-called Firsov plane dividing the ion and atom in the quasi-molecule, the energy loss to electrons per collision with one atom is

Chapter 1. Particle-solid interactions and radiation eects given by: Te= 0.35(Z1+ Z2)5/3~/a0 [1 + 0.16(Z1+ Z2)1/3b/a0]5 v (1.26)

where ~ is the reduced Planck constant. Since the energy transfer Teis impact parameter

b dependent, by inserting Eq.(1.26) into Eq.(1.16) and performing integration on b, one can get the electronic stopping power which exhibits a similar form to that of the Lindhard one. The main dierence between the two models comes from the dierent interatomic potentials used.

Ions with high energies

If the ion velocity is larger than v0Z 2/3

1 , the ion can be considered as a bare nucleus,

and its interactions with (supposedly free) target electrons can be accurately described by a pure Coulomb interatomic potential. Although the term of electronic stopping is often connected with inelastic collisions, interactions in the high energy region can be treated by an elastic approach introduced previously, i.e., the impulse approximation.

Inserting the Coulomb potential to Eq.(1.20), the energy transferred to an electron in a collision is given by:

Te =
4p2
2me
= 2Z
2
1e4
b2_{m}
ev2
(1.27)
Once again, according to Eq.(1.16), the electronic stopping power can be obtained as
follows:
dE
dx
e= ne
Z bmax
bmin
Te2πbdb =
4πZ_{1}2e4ne
mev2
lnbmax
bmin
(1.28)
In Eq.(1.28), the minimum impact parameter bmin is related to the maximum transferred

energy Tmax according to Eq.(1.27). Since me M1, Tmax can be represented by 2mev2,

and the bmin is derived as:

bmin =

Z1e2

mev2 (1.29)

The maximum impact parameter bmax is related to the minimum transferred energy,

Tmin, which a target-atom electron can accept. Tmin can be represented by the average

excitation energy of an electron, I. Hence, bmax is derived as:

bmax=

2Z1e2

(2mev2I)1/2

(1.30)

Substituting Eq.(1.29) and Eq.(1.30) into Eq.(1.28), and considering a correction due to distant resonant energy transfer, the electronic stopping power can be expressed as:

dE
dx
e
= 2πZ
2
1e4
E0
N Z2
M_{1}
Me
ln2mev
2
I (1.31)

Chapter 1. Particle-solid interactions and radiation eects

The average excitation energy I, in eV, for most elements is roughly 10Z2 [57].

It can be found that, in the high energy region, the electronic stopping power is
inversely proportional to v2 _{(or E}

0), which exhibits an opposite trend compared to the

stopping power in the low energy region. After taking into account the corrections for relativistic terms and for the non-participation of the strongly bound inner shell electrons, Eq.(1.31) can be transformed into the Bethe formula.

Empirical approach

In order to accurately describe the electronic stopping powers of ions in both the low and high energy regions, empirical approaches, for example, the one used in SRIM, can be applied. Ziegler et al [59] collected a data base of H electronic stopping cross sections, SH,

from experimental measurements of both H and He ions in solids. Then, the electronic stopping cross sections for heavy ions, SHI, can be obtained from SH at the same velocity

using the scaling rule [78]:

SHI = SH(ZHI∗ )
2 _{= S}

HZHI2 γ

2 _{(1.32)}

where ZHI is the atomic number of the heavy ion, ZHI∗ = ZHIγ is the eective charge of the

heavy ion, and γ is its fractional eective charge obtained based on the Brandt-Kitagawa (BK) theory [79].

An example of an electronic stopping power calculated from SRIM, i.e., the stopping power of He ions in UO2, is shown in Fig.1.2. Compared to the nuclear stopping power,

the electronic stopping power dominates the total stopping when the ion energy is high. In addition, there are also other available stopping data, for example, the data used in the RUMP code [80]. Fig.1.2 also shows the electronic stopping power calculated from RUMP in the energy range of 100 keV to 3.5 MeV which corresponds to the lower cuto and upper t energies in that code [81]. It is found that the RUMP data provides more accurate descriptions of the electronic stopping power of He ions in UO2 based on RBS

experiments. One reason is that there may be anomalously lower energy loss to materials
with a band gap due to fewer energy excitation levels available, and experimental data
indicates that the electronic stopping power is proportional to v0.7 _{instead of v in Si and}

Ge in the low energy region [59]. Indeed, according to the least square t, Fig.1.2 shows
that the RUMP stopping power is proportional to v0.6 _{in the energy range of 100 keV to}

250 keV (corresponding to the velocity of v0Z 2/3

1 ), which is close to that of Si and Ge.

In contrast, the electronic stopping power calculated by SRIM is roughly proportional to v in the low energy region, where the electronic stopping power increases with the He energy.

Chapter 1. Particle-solid interactions and radiation eects

### 1.2 Other particle-solid interactions

Apart from ion irradiations, neutron, electron and photon irradiations can often be found in harsh environments, such as nuclear reactors. Thus, it is pertinent to briey discuss their interactions with solid materials. Some insights on these interactions can be readily obtained by applying the methods used to treat ion-solid interactions.

### 1.2.1 Neutron irradiations

Since neutrons have no electric charge, they can directly interact with target nuclei. Among various types of interactions with nuclei, the elastic scattering, i.e., the (n, n) reaction, is one of the major sources of radiation damage found in reactor structural materials. If the classical mechanics depicted in Sec.1.1.1 are applied to treat such an elastic scattering, the Coulomb potential needs to be changed to a hard-sphere potential:

V (r) =
∞ _{, r 6 R}
0 , r > R (1.33)
where the parameter R represents the sum of the neutron and the nucleus radii, which is
also equal to the distance of closest approach, rmin. Since the same energy and momentum

conservation laws can be used, the transferred energy T is still given by Eq.(1.3). The relation between the impact parameter b and the scattering angle θc is represented by:

b = rmincos

θc

2 (1.34)

Inserting Eq.(1.34) into Eq.(1.13), the angular dierential cross section is obtained as: dσ(θc)

dΩ = r2

min

4 (1.35)

And the energy transfer dierential cross section can be generated by using Eq.(1.15):

dσ(E) = πr

2 min

TM

dT (1.36)

From these new equations obtained by using the hard-sphere potential, we can nd distinct dierences between the neutron and ion irradiations:

1. The angular distribution of scattered neutrons is isotropic 6_{, and the probability}

of energy transfer is constant over the range 0 to TM. In contrast, small-angle

6_{Actually, with the increase of neutron energy (> 1 MeV), the scattering becomes more forward [}_{82}_{].}
More accurate calculations can be performed using the optical model for nuclear scattering [83].

Chapter 1. Particle-solid interactions and radiation eects

scatterings are dominant in ion-solid interactions. Therefore, the spectrum of the
transferred energy from neutron irradiations due to elastic collisions is harder than
that from ion irradiations7_{;}

2. By integrating Eq.(1.35), the total neutron elastic scattering cross section can be calculated as πr2

min. Then, we can estimate that the mean free path between two

collisions, 1/(Nπr2

min), is on the order of magnitude of 0.1 m, which is way larger

than the typical range(∼ µm) in ion irradiation processes.

In terms of other reactions, for example in radiative captures, i.e., (n, γ) reactions, the energy T from the emission of a single γ photon of energy Eγ (Eγ < Q, where Q is the

energy released from nuclear reactions) is given by [82]:

T = E

2 γ

2Mdc2

(1.37)

where Mdis the mass of the daughter nucleus (recoil nucleus). In general, (n, γ) reactions

lead to rather small T since the photon cannot carry away very much momentum [84]. In addition to radiative captures, nuclear ssions could be interesting reactions to mention, since UO2 is used as an example material in this thesis. Usually, the ssion reaction can

be represented by:

235

U + n →236U∗ →Ad1_{X}

d1+Ad2Xd2+ 2.42n + Q (1.38)

where 236_{U} _{is on the excited state, 2.42 is the average number of prompt neutrons}

generated8_{, X}

d1and Xd2are two daughter nuclei with their mass numbers as Ad1and Ad2,

respectively. The daughter nuclei are not determined uniquely, and they usually consist of one light and one heavy nuclei with the most probable mass numbers as 95 and 140, respectively. The average Q released from the ssion is around 200 MeV, and roughly 80 % of the ssion energy becomes kinetic energy of the daughter nuclei. The most probable T to the light and heavy daughter nuclei are 98 MeV and 66 MeV, respectively, which will be further transferred to target atoms through ion-solid interactions. The remaining energy is shared by neutrons, γ rays, β and γ decays of daughter nuclei [85].

Generally, neutron reactions can be quite complex. In practice, for example, in representative neutron transportation codes, e.g., the MCNP [86] and TRIPOLI [87] codes, detailed data like reaction cross sections are extracted from nuclear data libraries, such as the ENDF/B library [88].

7_{A harder spectrum indicates that there are more neutrons or ions in high energy regions.}

8_{The prompt neutrons are emitted at the instant of ssion (within 10}−16 _{s), which is in contrast to}
delayed neutrons emitted following the β decay of the ssion fragments.

Chapter 1. Particle-solid interactions and radiation eects

### 1.2.2 Electron and photon irradiations

In electron irradiations, both elastic collisions with target atoms and inelastic scatterings can take place. In Sec.1.1.2, we already mentioned the collision of an electron at rest with an ion of high velocity. However, if we want to study the interaction in a reciprocal way, i.e., the interaction of a moving electron with an atom at rest, there will be noticeable dierences mainly due to the very small mass of an electron compared to that of an ion:

1. In many electron irradiation conditions, the relativistic eect may not be negligible (for example, when the electron energy is 100 keV, it already has a speed of 0.55c). In these conditions, the transferred energy in elastic collisions can still be described by T = TMsin2(θc/2), but TM must be adjusted to:

TM =

2Ee(Ee+ 2mec2)

M2c2

(1.39)

where Ee is the electron kinetic energy, me and M2 are rest masses of electrons and

target atoms, respectively [89].

2. Accelerated charged particles can give rise to bremsstrahlung. Compared to ions, electrons are signicantly aected by such radiative process of energy loss at much lower energy. Therefore, when the electron energy is high, the stopping power is contributed by collisions as well as by the energy loss due to bremsstrahlung. The critical energy at which the two stopping terms are equal can be obtained as follows[90]:

Ec≈

1600mec2

Z2 (1.40)

It can be found that Ec decreases with a higher Z2. Hence, high Z materials are

not preferred in shielding β radiations.

For photon irradiations, we mainly refer to X-rays or γ-rays radiations. These photons interact with solids mainly through three processes, which leads to the emission or generation of electrons:

1. Photons can transfer their energy, Ep, to electrons in the vicinity of an atom through

the photoelectric eect. In this process, the kinetic energy received by the so-called photoelectron, Te, is given by:

Te= Ep− Eb (1.41)

where Eb is the binding energy of the electron. In the lling process of the vacancy

left by the photoelectron, additional energy can be released, which can further induce the emission of either characteristic X-ray photons or Auger electrons.

Chapter 1. Particle-solid interactions and radiation eects

2. The photon can inelastically scatter with a (free) electron by Compton scattering, after which the wavelength of the scattered photon becomes larger. By applying relativistic kinematics and conservation of total energy and of momentum, the scattered photon energy is given by [91]:

E_{p}0 = Ep

1 + (Ep/mec2)(1 − cos θ)

(1.42)

Then, the kinetic energy of the scattered electrons is calculated as Te = Ep− Ep0.

3. If a photon is in the vicinity of an atom, the photon with its entire energy can be converted into an electron-positron pair by pair productions. There exists an energy threshold of 1.022 MeV for this process. Following the annihilation of the positron, two photons, each with an energy of 0.511 MeV, are created, which may further interact through the photoelectrical process or Compton scattering [83].

In addition, photons can also experience elastic scattering with free electrons through Thomson scattering, in which the wavelength of the photons does not change. Although this process generates little eect on targets, it is the basis for one of the methods used to characterize radiation damage in this thesis, i.e., the XRD method. Following classical theories, if an unpolarized beam with the intensity as I0 is scattered by a single

free electron, the intensity of the scattered beam, I, can be calculated by the Thomson
scattering equation:
I = I0
e4
m2
ec4R2
1 + cos2_{φ}
T
2
(1.43)
where the I is measured at a distance R from the electron at an angle φT with the incident

beam direction and the last term, (1 + cos2_{φ}

T)/2, is the polarization factor[92].

### 1.3 Radiation eects

Radiation eects basically stem from the change of target atomic structures. In elastic collisions, the energy transferred from incident particles provides the impetus for displacing target atoms. The displaced atoms may form stable defects which can undergo evolutions as a function of time and projectile particle uence. As a direct result of particle-solid interactions, the generation of stable defects from displaced atoms is referred to as the primary radiation damage. In this section, we will present basic mechanisms related to primary radiation damage, which is followed by the description of defect evolution. Other eects due to the introduction of foreign atoms and electronic stopping, which are mainly found in ion-solid interactions, will be mentioned at the end of the section.

Chapter 1. Particle-solid interactions and radiation eects

### 1.3.1 Primary radiation damage

In the framework of elastic collisions, a target atom can be permanently displaced from its original position if the transferred energy T is larger than the threshold displacement energy, Ed. Typical values of Ed, depending on materials, vary from 20 to 100 eV [93]. In

the process of irradiation, the target atom permanently displaced by a projectile particle is called the primary knock-on atom (PKA). Displaced atoms (or recoils) including PKAs can in turn displace other atoms, by which way a collision cascade is formed. Fig.1.4 shows an example of collision cascades created by 4 MeV Au ions in MgO according to SRIM simulations. Collision cascades containing less than 200 recoils are represented by grey spheres, and those having more than 200 recoils are represented by other colors. Fig.1.4 indicates that an energetic particle can generate numerous collision cascades with dendritic shapes, in which a large branch can have small sub-branches, resembling a fractal structure. In terms of radiation damage, the number of displacements in all the collision cascades has drawn particular attention shortly after the advent of nuclear reactors in the 1940s [94], and various methods for calculating this value have been proposed.

Figure 1.4 Collision cascades created by 4 MeV Au ions in MgO simulated by SRIM using the full damage cascades mode. The grey spheres indicate the collision positions involved in collision cascades in which the total number of recoils is less than 200. For collision cascades containing more than 200 recoils, the collision positions are indicated by other colors. (Insets show a collision cascade induced by a PKA with 47.5 keV energy and another one induced by a PKA with 41.4 keV energy. Ed(M g) = Ed(O) = 60

Chapter 1. Particle-solid interactions and radiation eects

Calculation of displacements

Before an accurate picture of stopping power was established, the well-known analytical model for estimating the average number of displacements, < Nd(E) >,

produced by a projectile with an energy E, was proposed by Kinchin and Pease (KP) in the 1950s [95]. Based on binary elastic collisions between like atoms and using a hard sphere interatomic potential, < Nd(E) > can be calculated as follows:

< Nd(E) >= 0, if E < Ed 1, if Ed6 E < 2Ed E/2Ed, if 2Ed6 E < EKP EKP/2Ed, if E > EKP (1.44)

where EKP is an energy limit depending on the properties of both projectile and target

atoms, above which all the energy is lost in inelastic interactions, and below which the electronic energy loss is neglected. It has been shown that this form of function can be reached based on dierent arguments. One method is to rstly assume a conservation of displacement:

< Nd(E) >=< Nd(E − T ) > + < Nd(T ) > (1.45)

in which < Nd(T ) >is the average displacements induced by recoils with an energy T , and

< Nd(E − T ) > is the average displacements created by the scattered projectile. Then,

the < Nd(E) > in the KP model can be obtained from the following integral equation:

< Nd(E) >=

Z T

0

[< Nd(E − T ) > + < Nd(T ) >]P (E, T )dT (1.46)

where P (E, T ) is the probability density of transferring energy T . For elastic collisions using a hard sphere potential, the probability density just equals to (1/E).

The KP model exhibits a quality of conciseness, but it suers from non-negligible discrepancies with experimental results. Therefore, two important improvements of the KP model have been made:

1. The hard sphere potential was replaced by a more realistic one, that is, a potential varying as an inverse power of the transferred energy T [96]. This improvement can be represented by multiplying the original equation with a constant ξ, which is smaller than 1. It is because a more realistic potential prefers forward-scattering (T E), which leads to a higher portion of energy spent in subthreshold collisions than hard-sphere scattering [97]. Both analytical theory and computer simulations suggest ξ near 0.8 [98].

Chapter 1. Particle-solid interactions and radiation eects

2. The energy E can be replaced by the so-called damage energy, ν(E), which is the amount of PKA energy not given to electrons. For collisions between like atoms (Z1 = Z2), Lindhard et al. [99] proposed the damage energy as follow:

ν(E) = E

1 + kg(ε) (1.47) where k is related to the Lindhard electronic stopping cross section, g(ε) is a function of the reduced energy ε (The exact expressions of k, ε and g(ε) can be found from relevant literatures [57]).

Applying above improvements, we can get < Nd(E) > from the so-called modied KP

model or the Norgett, Robinson and Torrens (NRT) model:

< Nd(E) >= 0, if E < Ed 1, if Ed 6 E < 2.5Ed 0.8ν(E) 2Ed if 2.5Ed6 E < ∞ (1.48)

Alternatively, < Nd(E) >can be obtained from binary collision approximation (BCA)

simulations, which is argued to be more "correct" than using the analytical models9 _{due}

to the following reasons: (i) the BCA simulations can take into account the collisions between dierent atoms (Z1 6= Z2, M1 6= M2); (ii) more accurate electronic stopping

powers can be used in the simulations, like the one used in SRIM. However, the stochastic treatment applied in the BCA simulations cannot relieve the situation encountered by the analytical models. In general, the dpa calculated with the NRT model (dpa can be obtained by dividing the displacement number by the total number of target atoms in the damaged region), for example, in metals, tends to overestimate the number of stable defects by a factor of 3 to 4 [100].

The salvation has long been considered to be the integration of the recombination eects. Based on the BCA simulations, Robinson and Torrens proposed a vacancy capture radius, rv. Only when the distance between the target atom original location and its rest

location after the collision is larger than rv, a stable defect forms. Thus, < Nd(E) >

can decrease by increasing rv [101]. Recently, Nordlund et al. [100] proposed a modied,

more sophisticated disorder parameter, based on the dpa denition, that is called athermal recombination corrected dpa (or arc-dpa). In this description, a defect surviving fraction, ξsurvive, is multiplied with < Nd(E) > calculated by the NRT model. Their argument is

similar to that of Robinson, which states that only defects far from the cascade center

9_{It is more correct in terms of the physical treatment, but the discrepancy with experimental values}
could be larger.

Chapter 1. Particle-solid interactions and radiation eects

can survive. Fitting parameters in ξsurvive need to be determined from MD simulations

or experiments. Since the < Nd(E) > value depends on the method used, it has been

appealed that when the displacement value is reported, the method used to estimate it should be clearly stated [102,103].

In general, the NRT model or the approach based on the BCA simulations are of importance credited to their broad adoptions in various materials. However, the whole process of recombination cannot be embedded in, and the term "displacement" conceals the various nature of the generated defects. Therefore, an alternative description is needed to better understand the generation of primary radiation damage.

Cascade evolutions

Generally, the stage of primary radiation damage lasts around 10 ps [104], which is too
short to be observed experimentally. On the contrary, the cascade phenomenon can be
caught by MD simulations. The cascade development can be separated into the collision
phase and the thermal spike (or heat spike, or displacement spike [105]) phase [106]10_{. In}

the collision phase, the PKA energy is distributed among atoms through collisions, which creates highly disordered regions. The number of displacements increases sharply until a maximum displacement is reached, which occurs in around 0.1 to 1 ps, depending on the PKA energy. In the thermal spike phase, the PKA energy shared among numerous atoms is dissipated through lattice vibrations. At the beginning of this second phase, the density of deposited energy in the disordered region is so high that local melting can occur [107]. Then, the thermal spike undergoes a quick cooling down period, which can be considered as a recrystallization process of hot liquid. During this recrystallization (or recombination) process, the majority of displaced atoms return to regular lattice sites. When the disordered region regains thermal equilibrium with the bulk at the end of thermal spike, only a fraction of displacements survive, which constitutes stable defects. In general, the number of stable defects, NM D

d , is smaller than the number of displacements

calculated by the NRT model, NN RT

d , and the ratio of NdM D to NdN RT decreases with

energy until the onset of subcascade formation [104]11_{.}

As an example, Fig.1.5 shows the development of a collision cascade induced by a 2.46 keV Si PKA in 3C-SiC at 300 K, according to a MD simulation. The simulation was performed with a 30a × 30a × 30a SiC cell containing 216000 atoms using the LAMMPS code [109,110] (a is the lattice parameter of 3C-SiC). The Terso/ZBL style potential [111]

10_{Note that there is a dierent meaning for the term of "thermal spike" when it is used in case of}
irradiation with high energy ions, in which the ion energy is mainly dissipated by electronic excitations.

11_{Recently, it is found that the ratio of N}M D

d to NdN RT in alloys could continue to decrease even after the subcascade formation, when the PKA is a light constituent atom in the alloy [108].

Chapter 1. Particle-solid interactions and radiation eects

was used to describe the interactions between atoms, and periodic boundary conditions were applied in all directions. The number of particles, volume and energy (NVE, a microcanonical ensemble) in the cell were kept constant. A kinetic energy of 2.46 keV was imparted to a Si atom in the bulk region to initiate the collision cascade. In order to prevent shock waves or thermal energies re-entering the cell through periodic boundaries, the velocities of atoms in the boundary layers, with a width of 2a, are scaled to that corresponding to 300 K [12]. In Fig.1.5.(a-f), the vacancy and interstitial pairs as well as antisites were analyzed with the Wigner-Seitz cell method using the OVITO software [112]; in Fig.1.5.(g-h), the potential energy of each atom was calculated by the LAMMPS code. The simulation shows that the number of vacancy and interstitial pairs reaches a maximum, which is 67, at around 0.1 ps, and then starts to decrease. The number of antisites exhibits a similar trend, but with a longer time to reach the maximum. After around 1 ps, the total number of defects becomes stable; compared to the maximum number, 54 % of vacancy and interstitial pairs survive from recombinations, which become stable Frenkel pairs; the dominant defects are Frenkel pairs and the rest are antisites. Both the gures of defects and plots of potentials indicate that there seem to be the formation of subcascades.

The displacements surviving the recrystallization process can have various types. Some defects and the associated formation mechanisms are described hereafter:

• Frenkel pairs: A Frenkel pair is formed if a vacancy and an associated interstitial are separated by a minimum distance that prevents their recombination [113]. In the MD simulations of collision cascades in Cu [107], it is found that only interstitials escaping from melted regions can survive. With a higher PKA energy, the melted region will be larger, and the survived fraction can be smaller. Therefore, the ratio of NM D

d to N N RT

d tends to decrease with a higher PKA energy, until the formation

of subcascades.

• Vacancy clusters: Vacancies left in a melted region can be pushed towards the
center region by the recrystallization front, as shown in MD simulations performed
in Co/Cu bilayer cells [114]. Thus, vacancies are able to meet and form clusters 12_{.}

• Interstitial clusters: In a collision cascade, if the melted region has an elongated shape, the recombination of excess interstitials in the tip and vacancies in the center can be prevented by the recrystallization occurring between the tip and the center, which traps the excess interstitials and generates clusters. Such mechanism is called the "liquid-isolation" mechanism, which is observed in Pt [115]. There is

Chapter 1. Particle-solid interactions and radiation eects

(a) (b) (c)

(d) (e) (f)

(g) (h) (i)

Figure 1.5 Collision cascade in 3C-SiC induced by 2.46 keV Si PKA. (a)-(f) show interstitial (blue) and vacancy (orange) pairs, and antisites (red) at 0.012, 0.048, 0.098, 0.200, 1.200 and 11.200 ps respectively. (g)-(i) show atoms in a layer, with the width as 2a (a is the lattice parameter), aected by the collision cascade at 0.048, 0.098 and 11.200 ps respectively, in which the potential energy of each atom is presented by the color bar legend ranging from -7 eV to -3 eV.

also another mechanism proposed for the formation of large clusters, which is due to the interaction of shock waves [116].

• Dislocation loops: Both interstitial-type and vacancy-type dislocation loops are

Chapter 1. Particle-solid interactions and radiation eects

found in high-energy collision cascades, for example, cascades induced in W [117] and Fe [118]. It can be argued that if the total kinetic energy imparted to clusters is high enough, there is a possibility for the formation of dislocation loops due to the collapse of clusters.

• Amorphous clusters: The formation of amorphous clusters are observed in semiconductors, e.g., Si and Ge [115]. The reason is attributed to the relatively weaker defect annealing in semiconductors compared to that in metals, due to dierent types of bonds [119].

### 1.3.2 Defect evolution and other radiation eects

Defect evolution

After primary damage events are formed, in the time scale of ∼ 10 ps, mobile defects
can diuse and interact with each other and/or with other defects, which eventually
decides the form of the radiation defects observed experimentally 13_{. For example,}

both vacancies and/or self interstitial atoms (SIAs) are highly mobile at temperatures of practical interest [121]. Vacancies and interstitials can annihilate upon meeting each other, or they can be absorbed by defect sinks, such as dislocations, voids, free surfaces, etc. Such diusion is usually accomplished by the interchange between atoms and neighboring point defects in a random way, and the diusion coecient, D, of a target atom is described as follows:

D = fvDvCv + fiDiCi+ f2vD2vC2v+ · · · (1.49)

where f is a correlation factor close to unity, C is the defect concentration, the subscripts v, iand 2v represent vacancy, interstitial and di-vacancy, respectively. Since irradiation can introduce point defects whose concentrations are much larger than the thermal equilibrium concentrations, D can be increased by irradiation. As a result, the diusion is enhanced by radiation [122]. In general, the timescale of defect evolution due to diusion exceeds the one that can be handled by MD simulations. The task of handling such defect evolution can be tackled by using methods like RE or KMC, as mentioned in the introduction part. The diusion of defects could play a crucial role in the accumulation of damage. For example, simulations based on the RE method reveal that, when the temperature is increased, an asymmetry in the vacancy and interstitial migration energies leads to a delayed damage accumulation, as observed in MgO, in contrast to c-ZrO2 for which both

migration energies are similar and the disordering process is accelerated [123].

13_{If the defect mobility is strongly limited, it seems that primary defects can also be directly observed}
in dedicated experiments, such as in the experiment of self-ion irradiation of W at cryogenic temperature
[120].